Electronic Supplementary Information file for article: Electronic Supplementary Information file for...
Embed Size (px)
Transcript of Electronic Supplementary Information file for article: Electronic Supplementary Information file for...
Electronic Supplementary Information file for article:
XANES study of Vanadium and Nitrogen dopants in photocatalytic TiO2 thin films
Zakaria El Koura, Giacomo Rossi, Marco Calizzi, Lucia Amidani, Luca Pasquini, Antonio Miotello, Federico Boscherini
EXPERIMENTAL AND THEORETICAL METHODS
Sample preparation and characterization
Before each deposition, a base pressure of about 10-7 mbar was achieved in the deposition chamber
of the RF-sputtering and the target was pre-sputtered for 20 minutes to remove all possible
contaminants from the surface. The target-substrate distance was kept constant at 6.0 cm, and the
substrate holder was kept oscillating in the plasma to improve the homogeneity of the films.
X-ray absorption spectroscopy measurements and data analysis
In the measurements at the BM23 beamline, the incident energy was selected using a double bounce
flat crystal Si (111) monochromator. The Vortex Si drift diode detector was placed in the horizontal
plane at right angles to the impinging beam.
The following reference compounds (Ti and V oxides) were measured in transmission mode using
finely ground powders dispersed in polyethylene:
TiO2 anatase, Alfa Aesar, 99.6% (code: 36199)
TiO2 rutile, Alfa Aesar, 99.99% (code: 14631)
V2O3, Sigma-Aldrich, 99.99% (code:463744)
VO2, Alfa Aesar, 99% (code: 22957)
V2O5, Sigma-Aldrich, 99.6 % (code: 221899)
For High Energy Resolution Fluorescence Detected (HERFD) XANES measurements at ID26
beamline, the V K fluorescence (4952.2 eV) from the samples was selected and focused on an
avalanche photodiode (APD) by five spherically bent (R = 1 m) Ge crystals in (331) reflection. The
incident energy was selected by the Si (311) reflection of a double crystal monochromator, and higher
harmonics were rejected by three Si mirrors under total external reflection.
For the processing of EXAFS spectra using Athena , the pre-edge region was fitted with a linear
function while the post – edge region was fitted with a spline to simulate the atomic cross section. As
a first approximation the energy origin for the energy – to – wavenumber conversion ( ) was chosen 𝐸0
as the maximum of the first derivative of the absorption spectrum.
Electronic Supplementary Material (ESI) for Physical Chemistry Chemical Physics. This journal is © the Owner Societies 2017
A state of the art EXAFS analysis at the Ti K-edge including multiple scattering (MS) contributions
was carried out on highly crystalline thin films and on reference anatase. Based on the
crystallographic structure, the single (SS) and MS contributions to the fine structure oscillations were
calculated using the FEFF code . Using ARTEMIS  the spectra were fitted excluding those
paths which gave a negligible contribution. Fitting parameters were an energy origin shift, a single
isotropic distance variation parameter and individual Debye – Waller (DW) factors for each path.
Spectra were fitted in the range and . We found that the following paths 𝑘 = 4.0 ‒ 11 Å ‒ 1 𝑅 = 1.1 ‒ 3.9 Å
were necessary for a meaningful fit: SS contributions related to the six O nearest neighbors (1st and
2nd shell, fitted as a single component in view of the small distance splitting) and the four Ti ions in
the 3rd and 4th coordination shell and a single three - legged MS contribution involving the O nearest
neighbors and the Ti in the 4th coordination shell. The path degeneracies were kept fixed at the values
of the crystals since, due to the well known high correlation with Debye – Waller factors, it was
impossible to determine them with a reasonable uncertainty.
Calculation of relaxed doped structures
Models for the local structure of doped TiO2 where obtained modifying rutile and anatase clusters.
Undoped crystal structures were obtained from literature . For the self-consistent field calculation
(SCF) we used Vanderbilt ultra-soft pseudopotentials  with the Perdew-Burke-Ernzerhof exchange
correlation functional  selected from the Quantum Espresso repository  (files Ti.pbe-sp-
van_ak.UPF, V.pbe-sp-van.UPF, N.pbe-van_ak.UPF and O.pbe-van_ak.UPF). The cutoff energy for
the wave functions of the plane wave algorithm was set to 30 Ry. The k space sampling was done
using a 4 x 4 x 4 mesh while the structural optimization was performed using the BFGS
algorithm [7,8] iterated until the total cluster force reached a value lower than . For one of 1 ⋅ 10 ‒ 3
the V-N-TiO2 models (M4), however it was impossible for us to achieve a total cluster force lower
than . This could be related to a higher instability of that configuration. 1 ⋅ 10 ‒ 2
In Table S1 we list the vector basis of the relaxed super cell structures compared to those of pure
anatase and rutile. The full atomic coordinate sets in Cartesian units are provided in a separate archive.
Supplementary Figures and Tables Table S1: Crystallographic parameters of relaxed doped super-cells. The * indicates pure compounds obtained joining multiple anatase and rutile unit cells.
Model a (Å) b (Å) c (Å) (°)𝛼 (°)𝛽 (°)𝛾
Anatase * 7.585 7.585 19.313 90 90 90
Rutile * 9.187 9.187 8.874 90 90 90
𝑉𝑇𝑖 7.585 7.585 19.313 90.00 90.00 90.00
𝑉𝑖 7.625 7.625 19.226 90.02 90.00 90.00
Model 1 7.606 7.575 19.281 90.00 89.99 90.00
Model 2 7.594 7.572 19.307 90.00 90.00 90.00
Model 3 7.563 7.575 19.439 89.86 90.04 90.00
Model 4 7.584 7.578 19.387 90.04 90.25 89.99
Model 5 7.597 7.592 19.372 90.00 90.00 90.00
Model 6 7.457 7.581 20.152 89.61 90.21 90.15
Model 7 9.279 9.279 8.904 89.99 89.99 90.42
Figure S1: Cross sectional SEM image of amorphous (a) and crystalline (b) V-TiO2 films.
Figure S2: Relaxed structures for V-doped and V-N-codoped TiO2. Ti in grey, V in yellow, O in red and N in blue. a: anatase TiO2; VTi : substitutional V in anatase; Vi : interstitial V in anatase;M1-M6: V-N-codoped anatase; M7: V-N-codoped rutile.
Table S2: Description of the starting and relaxed dopant configuration for all calculated models of V and N dopants in TiO2. Only model M7 refers to rutile, while the other models are for anatase. The images of the corresponding relaxed structures are displayed in Figure S2.
Model Label Starting configuration Relaxed configuration
VTi V substitutes Ti. V does not produce evident structural
distortions. The V-centered octahedron slightly shrinks
Vi V is placed in an interstitial site V reaches a stable position at the center of a
rhomboidal-based pyramid (Fig. S2-c)
M1 V substitutes Ti and N replaces one neighboring O The octahedron with the two dopants is
M2 V and N substitute Ti and O in different octahedra The dopant-containing octahedra are quite
similar to anatase
M3 V substitutes Ti. N is in an interstitial site near the V
N is attracted by the V octahedron and shares a corner with one O
M4 V substitutes Ti. N is in an
interstitial site far from the V octahedron
N is attracted by a Ti-centered octahedron and shares one corner with an O. Quite
unstable and difficult to relax
M5 V substitutes Ti. Far from the V dopant, a N2 dimer substitutes
one O in a Ti octahedron
The octahedron containing the two N atoms is slightly distorted compared to the anatase
M6 V substitutes Ti. A N2 dimer is placed in an interstitial site far
The N2 dimer is not split by the crystal field, while the surrounding crystal structure is
M7 V and N substitute Ti and O in two distant octahedra of the
The dopant-containing octahedra are quite similar to rutile
Table S3: Numerical results of quantitative EXAFS analysis carried out on reference anatase and V-
TiO2 crystalline thin films with different V content (2.4 and 4.5 at.% V). Numbers in brackets indicate
uncertainties in best estimates.
Anatase 2.4 at.% V 4.5 at.% V Path legs N R
(Å) σ2 (Å2) R
(Å2) O (1st/2nd)
2 6 1.9565 (99)
Ti (3rd) 2 4 3.055 (15)
Ti (4th) 2 4 3.804 (19)
O (1st/2nd) Ti (4th)
3 8 3.849 (20)
Figure S3: Magnitude of the Fourier Transform of Ti K-edge EXAFS spectra of the V-TiO2
crystalline thin films with different V content (1= 2.4 at.% V; 2= 4.5 at.% V), compared to reference
anatase (a). The Fourier transform was performed in the range with a weight. 𝑘 = 4.0 ‒ 11 Å ‒ 1 𝑘3
Dashed lines represent high quality fits.